# Correlation between temperatureâpressure dependence of the a ...

Correlation between temperatureâpressure dependence of the a ...

Correlation between temperatureâpressure dependence of the a ...

### Create successful ePaper yourself

Turn your PDF publications into a flip-book with our unique Google optimized e-Paper software.

Journal **of** Non-Crystalline Solids 351 (2005) 2616–2621

www.elsevier.com/locate/jnoncrysol

**Correlation** **between** temperature–pressure **dependence**

**of** **the** a-relaxation and configurational entropy

for a glass-forming polymer

Gustavo Ariel Schwartz a, *, Edurne Tellechea b , Juan Colmenero a,b ,Ángel Alegría b

a Donostia International Physics Center, Paseo Manuel de Lardizabal 4, 20018 San Sebastián, Spain

b Departamento de Física de Materiales UPV/EHU, Unidad de Física de Materiales CSIC-UPV/EHU, Facultad de Química,

Apartado 1072, 20080 San Sebastián, Spain

Available online 26 July 2005

Abstract

In this work we investigated **the** temperature–pressure **dependence** **of** **the** relaxation time **of** **the** a-relaxation process **of** poly(vinyl

acetate) (PVAc). By means **of** dielectric spectroscopy technique **the** relaxation time **of** **the** a-process was measured over a broad

range **of** frequencies (10 1 –10 7 Hz), pressures (0–300 MPa) and temperatures (320–460 K). Two different approaches were used

to analyze **the** temperature–pressure **dependence** **of** **the** relaxation time: **the** phenomenological Vogel–Fulcher–Tammann (VFT)

equation and **the** pressure extended Adam–Gibbs (PEAG) equation recently proposed. We compared both results and discussed

**the** validity **of** **the** VFT approach for PVAc at different pressures. We found an excellent agreement **between** **the** experimental data

and **the** PEAG equation, which only needs four parameters to describe **the** complete temperature–pressure **dependence** **of** **the** relaxation

time **of** **the** a-process. Finally, we showed that **the** **the**rmal and volumetric contributions to **the** configurational entropy are

clearly separated for PVAc.

Ó 2005 Elsevier B.V. All rights reserved.

PACS: 64.70.Pf; 77.22.Gm; 65.60.+a

1. Introduction

By cooling at sufficiently high rates many liquids do

not crystallize, becoming supercooled and finally enter

to **the** glassy state where **the** molecular motions **of** **the**

system are frozen in **the** time scale **of** **the** experiment.

Although **the** most common way to reach **the** glassy

state is by decreasing **the** temperature **of** **the** system,

**the** glass transition can also be approached by applying

high enough pressure to a supercooled liquid. Both

* Corresponding author. Tel.: +34 943 015 389; fax: +34 943 015

600.

E-mail address: schwartz@sw.ehu.es (G.A. Schwartz).

**the** increase **of** pressure and **the** decrease **of** temperature

result in slower molecular motions. These two different

ways **of** approaching **the** glass transition allow to

separate **the**rmal and volumetric effects and to reach a

better understanding **of** **the** glass transition process.

The temperature **dependence** **of** **the** relaxation time **of**

a supercooled liquid is usually described by **the** Vogel–

Fulcher–Tammann (VFT) [1–3] empirical equation

given by s(T) =s 0 exp(DT 0 /(T T 0 )). Although **the**

VFT **dependence** **of** **the** relaxation time with temperature

is, in general, in good agreement with **the** experimental

data, **the** lack **of** any clear physical

interpretation does not help in **the** understanding **of**

**the** nature **of** **the** glass transition. However, it has been

shown [4] that **the** temperature **dependence** **of** **the**

relaxation time expressed by **the** VFT equation can be

0022-3093/$ - see front matter Ó 2005 Elsevier B.V. All rights reserved.

doi:10.1016/j.jnoncrysol.2005.03.058

G.A. Schwartz et al. / Journal **of** Non-Crystalline Solids 351 (2005) 2616–2621 2617

derived, under certain assumptions, from **the** Adam–

Gibbs (AG) **the**ory [5] which is based on **the** concept

**of** **the** configurational entropy and allows linking **the**

dynamic and **the**rmodynamic behaviour **of** **the** glass

formers.

Additionally, **the** effect **of** pressure variation on **the**

dynamics **of** **the** a-relaxation process can be very useful

to investigate both **the**rmal and density effects. Some **of**

**the** seminal works in this area were done in **the** sixties

[6–8] and a renewed interest has arisen during **the** last

years [9–13]. The improvement **of** **the** experimental techniques

has made possible to obtain a large amount **of**

accurate data over broader ranges **of** pressure, temperature

and frequency and **the**refore contributes to **the** better

understanding **of** **the** involved processes. Thus, a new

equation describing **the** behaviour **of** **the** structural

relaxation time, s(T,P), as a function **of** both pressure

and temperature, has been recently proposed [10]. This

equation was derived from **the** Adam–Gibbs (AG) **the**ory

by writing **the** configurational entropy, S c , in terms

**of** **the** excess **of** both **the**rmal heat capacity and **the**rmal

expansion.

In this work **the** a-relaxation **of** poly(vinyl acetate)

(PVAc) was studied using dielectric spectroscopy

(10 1 –10 7 Hz) over a temperature range **between** 320

and 460 K and pressures up to 300 MPa. The temperature–pressure

**dependence** **of** **the** experimental a-relaxation

times was found to be very well described using

an extended AG equation [10] with **the**rmal and expansion

coefficients determined from calorimetric and PVT

data respectively.

2. Theory

The AG **the**ory, which is based on **the** assumption **of**

cooperatively rearranging regions, gives an expression

that relates **the** relaxation time with **the** configurational

entropy (S c ) [5]

C

s ¼ s 0 exp ; ð1Þ

TS c

where C is a material constant and S c is **the** configurational

entropy. However, since S c is not. accessible

experimentally, it is usually identified with **the** excess entropy

(S ex = S melt S crystal ). Although **the**re is still an

open debate about this point, some findings seem to suggest

a general validity **of** **the** proportionality **between** S ex

and S c [14]; under this assumption we identify S c with

S ex and **the**refore **the** proportionality constant **between**

**the**m will only affect **the** value **of** C in Eq. (1). Thus S c

can be estimated as [4]

S c ðT Þ¼ DH melt

T melt

Z T melt

T

DC P ðT 0 Þ

T 0 dT 0 ; ð2aÞ

where DC P ¼ C melt

P

would be **the** excess heat

capacity. In many polymers no melt is observed and a

C crystal

P

different procedure has to be followed to calculate S c .

Usually C crystal

P

is identified with C glass

P

and in order to access

**the** excess entropy what is calculated is

S c ðT Þ¼

Z T

T K

where DC P ¼ C melt

P

DC P ðT 0 Þ

T 0 dT 0 ; ð2bÞ

C glass

P

and T K is **the** Kauzmann

temperature, which used to be **of** **the** order **of** T g –

50 K, where **the** excess entropy would vanish. Generally,

an inverse temperature **dependence** is assumed for

DC P (DC P = K/T) and **the**refore, by integrating equation

(2b) and replacing S c in Eq. (1), withT 0 = T K , **the** VFT

expression for **the** temperature **dependence** **of** **the** relaxation

time is recovered. However, as we will see in this

work, this temperature **dependence** for DC P is not always

valid.

Recently, Casalini et al. [10] have proposed an extension

**of** **the** Eq. (2) for **the** configurational entropy (S c )

which also includes pressure as an independent variable

by adding a term related to **the** pressure change. Thus,

**the** temperature and pressure **dependence** **of** **the** S c is

given by

Z T

DC P ðT 0 Þ

S c ðT ; PÞ ¼g T ðPÞ

T K

T 0 dT 0 g P ðT Þ

Z P

D oV

dP 0 ;

0 oT

P 0

where

D oV

oT

P

¼ D oV melt

oT

P

D oV glass

oT

P

ð3Þ

ð4Þ

is **the** difference **of** **the** **the**rmal expansivity **of** **the** melt

and **the** glass; g T and g P are factors which could eventually

depend on pressure and temperature, respectively. If

**the**y are constant **the**n **the** **the**rmal and volumetric contributions

to **the** configurational entropy are very well

separated and **the**ir relative weights can be estimated.

In addition, if DC P follows a K/T law and g P /g T does

not depend on temperature a VFT behaviour is recovered

at any arbitrary fixed pressure with unique set **of**

values for s 0 and D. In this case we obtain **the** pressure

extended AG equation [11]

DT 0

sðT ; PÞ ¼s 0 exp

T T ; ð5Þ

0

T 0 ðPÞ ¼

1

g P

g T

1

S 1

T K

R P

0 D oV

oT

P 0 dP 0 ; ð6Þ

where s 0 , D and T K are **the** VFT parameters at atmospheric

pressure, and S 1 is **the** excess entropy at very

high temperature and atmospheric pressure.

2618 G.A. Schwartz et al. / Journal **of** Non-Crystalline Solids 351 (2005) 2616–2621

3. Experimental

3.1. Samples

Poly(vinyl acetate) (PVAc) (M w = 93080 g/mol) was

used for this study. The calorimetric glass transition

temperature, T g , was determined by differential scanning

calorimetry (DSC). The inflection point **of** **the** C P versus

temperature curve was 34.8 ± 0.1 °C.

3.2. Dielectric measurements under pressure

ε´´

2.0

1.5

1.0

0.5

P = 0.1 MPa

Dielectric measurements were carried out in a pressure

cell (0–300 MPa) supplied by Novocontrol GmbH.

The range 10 1 –10 5 Hz was measured with an EGG5302

lock-in amplifier in combination with a Chelsea dielectric

interface whereas for **the** range 10 3 –10 7 Hz a

HP4192LF impedance analyzer was used. A full description

**of** **the** experimental techniques can be found in reference

[13]. The sample measurements were performed

by frequency sweeps at constant temperature, with stability

better than ±0.1 K, and constant pressure, with

stability better than ±2 MPa.

a

ε´´

0.0

-1 0 1 2 3 4 5 6 7

Log(Freq[Hz])

2.0

T = 391.2K

1.5

1.0

4. Results and discussion

0.5

4.1. Dielectric relaxation spectra and relaxation times

Fig. 1a shows **the** dielectric loss (e 00 ), as a function **of**

frequency, under atmospheric pressure, at different temperatures

as determined using **the** pressure cell. Iso**the**rmal

spectra, at various pressures, are shown in Fig. 1b.

The central part **of** **the** main peak (i.e. **the** a-relaxation)

was described using **the** Alvarez–Alegría–Colmenero

function [15], which is a particular case **of** **the** Havriliak–Negami

(HN) function

e De

ðxÞ e 1 ¼

½1 þðixs HN Þ a Š ;

ð7Þ

b

where De is **the** relaxation strength, s HN is **the** relaxation

time and a and b are shape parameters with b ¼

1 0.812ð1 aÞ 0.387 . This last constraint allows reducing

**the** number **of** free parameters (without significant

decrease **of** **the** fitting quality) and also deducing from

this frequency domain fit **the** parameters **of** **the** corresponding

time domain Kohlrausch–Williams–Watts

(KWW) function [15].

Fig. 2 shows **the** Arhenius plot for **the** relaxation time

**of** maximal loss s ¼ s max ð¼ s HN ðsinðap=ð2 þ 2bÞÞÞ 1=b

ðsinðabp=ð2 þ 2bÞÞÞ 1=b Þ [16] at different pressures. Filled

and dashed lines represent **the** corresponding fits to **the**

phenomenological and **the**oretical predictions as explained

below. The experimental data are in very good

agreement with those previously published by OÕReilly

[6] and by Heinrich and Stoll [17].

b

0.0

0

1 2 3 4 5 6 7

Log(Freq[Hz])

Fig. 1. (a) Dielectric loss (e 00 ) at atmospheric pressure and different

temperatures (from left to right: 300.5, 313.5, 326.4, 339.4, 352.3,

365.3, 378.3 and 391.2 [K]). (b) Dielectric loss (e 00 ) at 391.2 K and

different pressures (from left to right: 300, 250, 200, 150, 100, 50 and

ffi0 MPa).

4.2. Phenomenological approach

Since **the** VFT equation has shown to be very useful

for an empirical description **of** **the** temperature **dependence**

**of** **the** relaxation times for several glass formers,

it is reasonable to use it as a first approximation. Actually,

some expressions, which are ÔnaturalÕ extensions **of**

**the** VFT equation, have been recently proposed [9,

18–20] to describe **the** temperature–pressure **dependence**

**of** **the** relaxation times. Phenomenological expressions

like

DðT 0 þ bP þ cP 2 Þ

sðT ; PÞ ¼s 0 exp

; ð8Þ

T ðT 0 þ bP þ cP 2 Þ

which is a particular case **of** Eq. (5), were found very

useful to fit **the** temperature–pressure **dependence** **of**

**the** relaxation time **of** several glass formers [11,21].

However, by keeping s 0 and D those determined from

atmospheric pressure, it is not possible to describe prop-

G.A. Schwartz et al. / Journal **of** Non-Crystalline Solids 351 (2005) 2616–2621 2619

log(τ[s])

erly **the** experimental data for PVAc by means **of** Eq. (8)

as shown in Fig. 2 for P = 300 MPa (dashed line). If we

leave s 0 as a free parameter, although **the** fitting is good,

s 0 varies more than one order **of** magnitude **between**

atmospheric pressure and 300 MPa which seems to be

unrealistic to our understanding. A possible explanation

for this atypical behaviour **of** PVAc could be related

with **the** strong decrease **of** DC P with temperature as reported

in **the** literature [22] and shown in Fig. 3. As

C P [J/K/mol]

2

0

-2

-4

-6

-8

-10

2.2 2.4 2.6 2.8 3.0 3.2

180

170

160

150

140

130

120

110

100

Amorphous

Crystal

1000/T [K -1 ]

Fig. 2. Relaxation time **of** **the** a-process **of** PVAc as a function **of**

inverse temperature at different pressures (from top to bottom: 300,

250, 200, 150, 100, 50 MPa, atmospheric pressure (ffi0 MPa)). Dashed

line corresponds to Eq. (8) with P = 300 MPa and s 0 and D those

determined from atmospheric pressure; **the** experimental data at

P = 0 MPa were fitted with both Eq. (10) and **the** VFT function (both

curves are overlapped in **the** figure); filled lines represent **the** predicted

values (see text) according to Eq. (13) (note that for P = 0 MPa

Eq. (13) reduces to Eq. (10)).

300 320 340 360 380 400 420 440

Temperature [K]

Fig. 3. Heat capacity (C P ) for both melt and crystal (taken from Ref.

[22]), and excess heat capacity ðDC P ¼ C melt

P

C crystal

P

Þ as a function **of**

temperature. The dashed line (with non-inverted triangles) represents

**the** extrapolated values **of** C crystal

P to temperatures above **the** glass

transition. The values **of** DC P (open circles) decrease linearly with

temperature as shown by **the** linear fit to **the** data. The thick line

represents **the** best fit **of** **the** DC P data to equation DC P = K/T.

45

40

35

30

25

20

15

10

5

∆C P

[J/K/mol]

aforementioned, what is generally assumed is that **the**

temperature **dependence** **of** DC P should be not far from

DC P = K/T which yield **the** VFT equation in **the** AG

framework. However, as shown in Fig. 3 **the** PVAc temperature

**dependence** **of** DC P is actually much stronger

than **the** K/T, which means that by using AG **the** VFT

equation is not recovered. As it was shown above, even

if **the** VFT is valid to fit **the** data at any fixed pressure, a

complete temperature–pressure description for **the**

relaxation time is not possible by using extensions **of**

**the** VFT equation like Eq. (8).

Taking all **the**se features into account we have

checked whe**the**r **the** extended Adam–Gibbs frame,

namely Eq. (3) in combination with Eq. (1), can provide

a full description **of** **the** temperature–pressure **dependence**

**of** **the** relaxation time.

Heat capacity and **the**rmal effects. Fig. 3 shows **the**

heat capacity (C P ) and **the** excess heat capacity (DC P )

for **the** PVAc in **the** temperature range **of** interest. It is

clear from this figure that DC P decreases in a nearly

linear fashion with temperature according to **the** empirical

equation DC P = b mT, where b = (103.96 ± 0.02)

JK 1 mol

1 and m = (0.21 ± 0.01) JK 2 mol

1 . According

with this, **the** **the**rmal contribution to **the**

configurational entropy would be

S c ðT ; P ffi 0Þ ¼g T

Z T

T K

DC P ðT 0 Þ

T 0 dT 0

¼ g T ðb lnðT =T K Þ mðT T K ÞÞ. ð9Þ

Thus, by introducing this result in Eq. (1), **the** temperature

**dependence** **of** **the** relaxation time at atmospheric

pressure would be given by

sðT ; P ffi 0Þ ¼s 0 exp

C=g T

T ðb lnðT =T K Þ mðT T K ÞÞ

ð10Þ

By using Eq. (10) to fit **the** experimental data we got

1

log(s 0 [s]) = 14.1 ± 0.1, C/g T = (99041 ± 540) Jmol

and T K = 255.5 ± 0.2 K.

It is interesting to note that even when **the** VFT equation

is not recovered from **the** AG **the**ory, it is still valid

as a phenomenological description **of** **the** experimental

data. Fig. 2 shows **the** best fit to **the** experimental data

(at atmospheric pressure) by using both Eq. (10) and

VFT equation with log(s 0 [s]) = 12.8 ± 0.1, D = 6.6 ±

0.1 and T 0 = 259.8 ± 0.1 K. The difference **between** both

curves is less than **the** width **of** **the** line and **the**refore

**the**y are superimposed in **the** figure.

Thermal expansion and volumetric effects. In order to

calculate **the** volumetric contribution to **the** configurational

entropy we need to estimate DðoV =oT Þ P

. The temperature

**dependence** **of** **the** volume was estimated by

plotting **the** specific volume for PVAc, as given in reference

[23], versus temperature and taking **the** slopes

below and above T g . For **the** different pressures **the** Tait

.

2620 G.A. Schwartz et al. / Journal **of** Non-Crystalline Solids 351 (2005) 2616–2621

∆(δV/δT) [cm 3 K -1 mol -1 ]

4.0

3.5

3.0

2.5

2.0

1.5

0 50 100 150 200 250 300

Pressure [MPa]

Fig. 4. D(oV/oT) P as a function **of** pressure. The data were fitted with

an empirical exponential function (see text).

equation [23] was used with **the** parameters reported in

[24] for **the** glassy state. Fig. 4 shows **the** pressure **dependence**

**of** DðoV =oT Þ P

so obtained and **the** best fit to an

empirical exponential decay according to

DðoV =oT Þ P

¼ DðoV =oT Þ P¼0

A½1 expð P=P 0 ÞŠ ð11Þ

with A = (2.15 ± 0.03)10 2 cm 3 K 1 mol

1 , P 0 = (129 ±

5) MPa and D(oV/oT) P =0 = (3.35 ± 0.03)10 2 cm 3 K 1

mol

1 . Therefore **the** pressure contribution to **the** configurational

entropy is

Z P

g P DðoV =oT Þ P 0dP 0 P

¼ g P P 0 DðoV =oT Þ P¼0

0

P 0

A P

þ expð P=P 0 Þ 1 .

P 0

ð12Þ

By using Eqs. (9) and (12) in Eq. (3) and **the**n by

replacing in Eq. (1) we have **the** following expression

for **the** temperature–pressure **dependence** **of** **the** relaxation

time

g P

/g T

1.4

1.2

1.0

0.8

0.6

0.4

0.2

0.0

more significant at high pressures, we estimated an average

value by weighting **the** data with **the** corresponding

pressure values. The solid line in Fig. 5 represents this

weighted average for all values. This is an important

result which shows that **the** temperature and pressure

contributions to **the** configurational entropy come exclusively

from **the** respective integrals in Eq. (3).

Once **the** value **of** g P /g T is known we can use Eq. (13),

with **the** parameters previously estimated at atmospheric

pressure (log(s 0 ),C/g T and T K ), to calculate **the** relaxation

time at any temperature and pressure. Fig. 2 shows

**the** excellent agreement among experimental data and

**the** predicted values (filled lines) for **the** relaxation time

using Eq. (13).

5. Conclusions

P = 50MPa

P = 100MPa

P = 150MPa

P = 200MPa

P = 250MPa

P = 300MPa

330 360 390 420 450

Temperature [K]

Fig. 5. Coefficient g P /g T as a function **of** temperature at different

pressures. Open symbols represent low pressure data whereas full

symbols are used for high pressure data. The line represents **the**

estimated constant weighted value (see text).

2

3

sðT ; PÞ ¼s 0 exp 4 nh

T bln T

T K

mðT

i

T K Þ

g P

g T

P 0

C=g

h T

D oV

oT

P

P¼0

io5. ð13Þ

P 0

A P P 0

þ expð P=P 0 Þ 1

Since we already know **the** values **of** log(s 0 ), C/g T and

T K , (determined from **the** fitting at atmospheric pressure)

we can use **the** experimental values **of** **the** relaxation

time to estimate g P /g T for different temperatures

and pressures. Fig. 5 shows g P /g T values versus temperature

for different pressures; no clear temperature or

pressure **dependence** is observed besides **the** experimental

uncertainties. Given that **the** effect **of** pressure is

We have shown that even if **the** phenomenological

VFT equation gives an excellent description **of** **the** temperature

**dependence** **of** **the** relaxation time at any given

fixed pressure, **the** complete description **of** **the** temperature–pressure

**dependence** is not possible by keeping s 0

constant. By leaving s 0 as a free parameter we got an

unreasonable change **of** s 0 with pressure.

The fit **of** experimental data with Eq. (13) shows not

only **the** validity **of** **the** AG frame but also that it is a

more general **the**ory which includes **the** VFT behaviour

G.A. Schwartz et al. / Journal **of** Non-Crystalline Solids 351 (2005) 2616–2621 2621

as a particular case. It is important to note that in

addition to **the** **the**rmodynamic data taken from **the**

literature, only four parameters are needed to fit s

(T, P): log(s 0 ), C/g T and T K (from P = 0 MPa data)

and g P /g T .

The fact that **the** value **of** g P /g T is constant is an indication

that **the**rmal and volumetric contributions to **the**

configurational entropy for PVAc are well separated

and **the**ir values are given by **the** integrals expressions

in Eq. (3).

Acknowledgements

This work has been supported in part by **the** Spanish

Ministry **of** Science and Technology (MICyT) (Project

MAT 2001/0070) and by **the** Government **of** **the** Basque

Country (Project 9/UPV 00206.215-13568/2001).

References

[1] H. Vogel, Phys. Z 22 (1921) 645.

[2] G.S. Fulcher, J. Am. Ceram. Soc. 8 (1923) 339.

[3] G. Tammann, W. Hesse, Z. Anorg. Allg. Chem. 156 (1926) 245.

[4] R. Richert, C.A. Angell, J. Chem. Phys. 108 (1998) 9016.

[5] G. Adam, J.H. Gibbs, J. Chem. Phys. 28 (1965) 139.

[6] J.M. OÕReilly, J. Polym. Sci. 57 (1962) 429.

[7] G. Williams, Trans. Faraday Soc. 62 (1966) 1321.

[8] G. Williams, Trans. Faraday Soc. 62 (1966) 2091.

[9] S. Corezzi, P.A. Rolla, M. Paluch, J. Ziolo, D. Fioretto, Phys.

Rev. E 60 (1999) 4444.

[10] R. Casalani, S. Capaccioli, M. Lucchesi, P.A. Rolla, Phys. Rev. E

63 (2001) 031207.

[11] D. Prevosto, M. Lucchesi, S. Capaccioli, R. Casalini, P.A. Rolla,

Phys. Rev. B 67 (2003) 174202.

[12] C.M. Roland, R. Casalini, Macromolecules 36 (2003) 1361.

[13] A. Alegria, D. Gomez, J. Colmenero, Macromolecules 35 (2002)

2030.

[14] C.A. Angell, S. Borick, J. Non-Cryst. Solids 307–310 (2002) 393,

and references **the**rein.

[15] F. Alvarez, A. Alegria, J. Colmenero, Phys. Rev. B 44 (1991)

7306;

A. H**of**mann, A. Alegria, J. Colmenero, L. Willner, E. Buscaglia,

N. Hadjichristidis, Macromolecules 29 (1996) 129.

[16] F. Kremer, A. Scöhnhals, Broadband Sielectric Spectroscopy,

Springer-Verlag, Berlin, 2003, page 64.

[17] W. Heinrich, B. Stoll, Colloid Polym. Sci. 263 (1985) 873.

[18] M. Naoki, H. Endou, K. Matsumoto, J. Phys. Chem. 91 (1987)

4169.

[19] C.A. Herbst, R.L. Cook, H.E. King, Nature 361 (1993) 518.

[20] J.T. Bendler, J.J. Fontanella, M.F. Shlesinger, Phys. Rev. Lett. 87

(2001) 195503.

[21] D. Gomez Plaza, PhD **the**sis, Univ. País Vasco, Spain, 2000.

[22] ATHAS database, http://web.utk.edu/~athas/databank/vinyl/

pvac/pvac.html U. Gaur, B. Wunderlich, J. Phys. Chem. Ref.

Data 10 (1981) 1051;

U. Gaur, B.B. Wunderlich, B. Wunderlich, J. Phys. Chem. Ref.

Data 12 (1983) 29.

[23] J.E. Mark, Physical Properties **of** Polymers Handbook, AIP Press,

New York, 1996, Chapter 7.

[24] J.E. Mc Kinney, R. Simha, Macromolecules 7 (1974) 894.